data_4329477
_audit_creation_method 'SHELXL-97'
_audit_creation_date	2023-11-06
_audit_update_record	2023-11-06
_database_code_COD	4329477
_journal_coden_ASTM	INOCAJ
_journal_year	2012
_journal_volume	51
_journal_page_first	6682
_journal_page_last	6686
loop_
_publ_author_name
'Jianxiu,,,, Zhang'
'Shufeng,,,, Zhang'
'Yicheng,,,, Wu'
'Jiyang,,,, Wang'

_publ_section_title
;
New Nonlinear Optical Crystal: NaBa4Al2B8O18Cl3








;
_chemical_formula_sum	'Al2 B8 Ba4 Cl3 Na O18'
_chemical_formula_weight	1107.140
_refine_ls_R_factor_all	0.060
_cell_length_a	12.0480(16)
_cell_length_b	12.048(2)
_cell_length_c	 6.8165(11)
_cell_angle_alpha	90.000
_cell_angle_beta	90.000
_cell_angle_gamma	90.000
_cell_volume	989.4(3)
_cell_formula_units_Z	2
_exptl_crystal_density_meas	3.700
_symmetry_cell_setting	tetragonal
_symmetry_int_tables_number	102
_symmetry_space_group_name_H-M	'P 42 n m'
_symmetry_space_group_name_Hall	'P_4n_-2n'

loop_
_symmetry_equiv_pos_site_id
_symmetry_equiv_pos_as_xyz
1 x,y,z
2 1/2-y,1/2+x,1/2+z
3 -x,-y,z
4 1/2+y,1/2-x,1/2+z
5 1/2-x,1/2+y,1/2+z
6 1/2+x,1/2-y,1/2+z
7 -y,-x,z
8 y,x,z

loop_
_atom_type_symbol
_atom_type_oxidation_number
_atom_type_radius_bond
Ba	?	?
Al	?	?
Na	?	?
O	?	?
Cl	?	?
B	?	?


loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_Wyckoff_symbol
_atom_site_attached_hydrogens
_atom_site_calc_flag
_atom_site_thermal_displace_type
_atom_site_u_iso_or_equiv
Ba1 Ba  0.9829(0)  0.7232(1)  0.2215(1)  1.000 8 d ? d Uani  0.0266(3)
Al2 Al  0.2979(2)  0.7021(2)  0.2133(8)  1.000 4 c ? d Uani  0.0111(6)
Na3 Na  0.0000  0.0000 -0.107(2)  1.000 2 a ? d Uani  0.049(3)
O1 O  0.1158(7)  0.7425(8)  0.5451(11)  1.000 8 d ? d Uani  0.0237(16)
O2 O  0.0627(6)  0.7980(6)  0.8691(11)  1.000 8 d ? d Uani  0.0175(14)
Cl1 Cl  0.0000  0.0000  0.2824(10)  1.000 2 a ? d Uani  0.0305(12)
Cl2 Cl  0.0000  0.5000  0.4488(16)  1.000 4 b ? d Uani  0.0589(19)
O5 O  0.3028(5)  0.6972(5)  0.4709(13)  1.000 4 c ? d Uani  0.0108(16)
O6 O  0.2002(6)  0.7998(6)  0.1242(13)  1.000 4 c ? d Uani  0.0145(18)
O7 O  0.2550(6)  0.7450(6) -0.2042(16)  1.000 4 c ? d Uani  0.0136(19)
B1 B  0.2335(11)  0.7665(11)  0.583(3)  1.000 4 c ? d Uani  0.017(3)
O8 O  0.4276(7)  0.7400(9)  0.1250(12)  1.000 8 d ? d Uani  0.0284(19)
B2 B  0.1854(8)  0.8146(8) -0.0800(19)  1.000 4 c ? d Uani  0.010(2)
B3 B  0.5326(9)  0.733(1)  0.1811(13)  1.000 8 d ? d Uani  0.013(2)



loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_site_symmetry_1
_geom_bond_site_symmetry_2
_geom_bond_distance
_geom_bond_publ_flag
Ba1 O1 . 1_655  2.736(8) no
Ba1 O2 . 1_654  2.740(8) no
Ba1 O7 . 2_655  2.818(7) no
Ba1 O6 . 1_655  2.854(4) no
Ba1 O8 . 6_565  2.865(8) no
Ba1 O5 . 2_654  2.924(6) no
Ba1 Cl2 . 1_655  3.111(6) no
Ba1 B1 . 2_654  3.151(14) no
Ba1 B3 . 6_565  3.233(9) no
Ba1 O1 . 2_654  3.240(9) no
Ba1 Cl2 . 2_654  3.276(6) no
Ba1 Cl1 . 1_665  3.3667(12) no
Al2 O8 . 7_665  1.735(9) no
Al2 O8 . .  1.735(9) no
Al2 O5 . .  1.758(10) no
Al2 O6 . .  1.772(10) no
Na3 O2 . 8_454  2.554(8) no
Na3 O2 . 1_544  2.554(8) no
Na3 O2 . 7_654  2.554(8) no
Na3 O2 . 3_564  2.554(8) no
Na3 Cl1 . .  2.657(17) no
Na3 B2 . 3_565  3.164(14) no
Na3 B2 . 1_545  3.164(14) no
O1 B3 . 6_465  1.396(12) no
O1 B1 . .  1.471(13) no
O1 Ba1 . 1_455  2.736(8) no
O1 Ba1 . 4_465  3.240(9) no
O2 B3 . 6_465  1.383(11) no
O2 B2 . 1_556  1.531(11) no
O2 Na3 . 1_566  2.554(8) no
O2 Ba1 . 1_456  2.740(8) no
Cl1 Ba1 . 8_445  3.3667(12) no
Cl1 Ba1 . 1_445  3.3667(12) no
Cl1 Ba1 . 3_665  3.3667(12) no
Cl1 Ba1 . 7_665  3.3667(12) no
Cl2 Ba1 . 3_665  3.111(6) no
Cl2 Ba1 . 1_455  3.111(6) no
Cl2 Ba1 . 4_465  3.276(6) no
Cl2 Ba1 . 2_545  3.276(6) no
O5 B1 . .  1.41(2) no
O5 Ba1 . 6_465  2.924(6) no
O5 Ba1 . 4_465  2.924(6) no
O6 B2 . .  1.415(16) no
O6 Ba1 . 7_675  2.854(4) no
O6 Ba1 . 1_455  2.854(4) no
O7 B2 . .  1.458(16) no
O7 B1 . 1_554  1.49(2) no
O7 Ba1 . 4_464  2.818(7) no
O7 Ba1 . 6_464  2.818(7) no
B1 O1 . 7_665  1.471(13) no
B1 O7 . 1_556  1.49(2) no
B1 Ba1 . 6_465  3.151(14) no
B1 Ba1 . 4_465  3.151(14) no
O8 B3 . .  1.325(14) no
O8 Ba1 . 6_464  2.865(8) no
B2 O2 . 1_554  1.531(11) no
B2 O2 . 7_664  1.531(11) no
B2 Na3 . 1_565  3.164(14) no
B2 Ba1 . 7_675  3.375(9) no
B2 Ba1 . 1_455  3.375(9) no
B3 O2 . 6_564  1.383(11) no
B3 O1 . 6_564  1.396(12) no
B3 Ba1 . 6_464  3.233(9) no

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_2
_geom_angle_site_symmetry_3
_geom_angle
_geom_angle_publ_flag
O1 Ba1 O2 1_655 . 1_654 118.3(2) no
O1 Ba1 O7 1_655 . 2_655 114.4(3) no
O2 Ba1 O7 1_654 . 2_655 117.1(3) no
O1 Ba1 O6 1_655 . 1_655 67.9(3) no
O2 Ba1 O6 1_654 . 1_655 50.8(2) no
O7 Ba1 O6 2_655 . 1_655 153.1(2) no
O1 Ba1 O8 1_655 . 6_565 49.4(2) no
O2 Ba1 O8 1_654 . 6_565 150.8(3) no
O7 Ba1 O8 2_655 . 6_565 65.1(3) no
O6 Ba1 O8 1_655 . 6_565 112.7(2) no
O1 Ba1 O5 1_655 . 2_654 151.4(2) no
O2 Ba1 O5 1_654 . 2_654 68.9(2) no
O7 Ba1 O5 2_655 . 2_654 48.5(3) no
O6 Ba1 O5 1_655 . 2_654 116.1(3) no
O8 Ba1 O5 6_565 . 2_654 109.7(2) no
O1 Ba1 Cl2 1_655 . 1_655 68.5(2) no
O2 Ba1 Cl2 1_654 . 1_655 134.2(2) no
O7 Ba1 Cl2 2_655 . 1_655 95.31(19) no
O6 Ba1 Cl2 1_655 . 1_655 109.54(19) no
O8 Ba1 Cl2 6_565 . 1_655 70.8(3) no
O5 Ba1 Cl2 2_654 . 1_655 128.59(19) no
O1 Ba1 B1 1_655 . 2_654 142.7(4) no
O2 Ba1 B1 1_654 . 2_654 93.4(4) no
O7 Ba1 B1 2_655 . 2_654 28.3(4) no
O6 Ba1 B1 1_655 . 2_654 142.4(4) no
O8 Ba1 B1 6_565 . 2_654 93.4(4) no
O5 Ba1 B1 2_654 . 2_654 26.4(4) no
Cl2 Ba1 B1 1_655 . 2_654 104.2(3) no
O1 Ba1 B3 1_655 . 6_565 25.3(2) no
O2 Ba1 B3 1_654 . 6_565 137.0(3) no
O7 Ba1 B3 2_655 . 6_565 89.1(3) no
O6 Ba1 B3 1_655 . 6_565 90.1(3) no
O8 Ba1 B3 6_565 . 6_565 24.1(3) no
O5 Ba1 B3 2_654 . 6_565 130.6(2) no
Cl2 Ba1 B3 1_655 . 6_565 69.3(3) no
B1 Ba1 B3 2_654 . 6_565 117.4(4) no
O1 Ba1 O1 1_655 . 2_654 145.5(3) no
O2 Ba1 O1 1_654 . 2_654 95.7(2) no
O7 Ba1 O1 2_655 . 2_654 45.9(3) no
O6 Ba1 O1 1_655 . 2_654 144.3(2) no
O8 Ba1 O1 6_565 . 2_654 102.9(2) no
O5 Ba1 O1 2_654 . 2_654 44.9(2) no
Cl2 Ba1 O1 1_655 . 2_654 83.97(17) no
B1 Ba1 O1 2_654 . 2_654 26.6(3) no
B3 Ba1 O1 6_565 . 2_654 125.5(2) no
O1 Ba1 Cl2 1_655 . 2_654 119.4(2) no
O2 Ba1 Cl2 1_654 . 2_654 75.5(2) no
O7 Ba1 Cl2 2_655 . 2_654 106.0(2) no
O6 Ba1 Cl2 1_655 . 2_654 94.35(17) no
O8 Ba1 Cl2 6_565 . 2_654 133.3(3) no
O5 Ba1 Cl2 2_654 . 2_654 89.10(18) no
Cl2 Ba1 Cl2 1_655 . 2_654 64.45(3) no
B1 Ba1 Cl2 2_654 . 2_654 85.6(3) no
B3 Ba1 Cl2 6_565 . 2_654 132.2(3) no
O1 Ba1 Cl2 2_654 . 2_654 60.94(15) no
O1 Ba1 Cl1 1_655 . 1_665 77.3(2) no
O2 Ba1 Cl1 1_654 . 1_665 76.2(2) no
O7 Ba1 Cl1 2_655 . 1_665 84.41(18) no
O6 Ba1 Cl1 1_655 . 1_665 69.66(17) no
O8 Ba1 Cl1 6_565 . 1_665 75.1(2) no
O5 Ba1 Cl1 2_654 . 1_665 78.04(17) no
Cl2 Ba1 Cl1 1_655 . 1_665 142.3(2) no
B1 Ba1 Cl1 2_654 . 1_665 93.2(3) no
B3 Ba1 Cl1 6_565 . 1_665 73.0(2) no
O1 Ba1 Cl1 2_654 . 1_665 119.52(16) no
Cl2 Ba1 Cl1 2_654 . 1_665 151.6(2) no
O8 Al2 O8 7_665 . . 110.8(7) no
O8 Al2 O5 7_665 . . 109.0(4) no
O8 Al2 O5 . . . 109.0(4) no
O8 Al2 O6 7_665 . . 107.7(4) no
O8 Al2 O6 . . . 107.7(4) no
O5 Al2 O6 . . . 112.7(5) no
O8 Al2 Ba1 7_665 . 7_675 152.3(4) no
O8 Al2 Ba1 . . 7_675 78.6(4) no
O5 Al2 Ba1 . . 7_675 91.2(3) no
O6 Al2 Ba1 . . 7_675 45.40(12) no
O8 Al2 Ba1 7_665 . 1_455 78.6(4) no
O8 Al2 Ba1 . . 1_455 152.3(4) no
O5 Al2 Ba1 . . 1_455 91.2(3) no
O6 Al2 Ba1 . . 1_455 45.40(12) no
Ba1 Al2 Ba1 7_675 . 1_455 82.31(7) no
O2 Na3 O2 8_454 . 1_544 124.1(4) no
O2 Na3 O2 8_454 . 7_654 172.8(8) no
O2 Na3 O2 1_544 . 7_654 55.4(4) no
O2 Na3 O2 8_454 . 3_564 55.4(4) no
O2 Na3 O2 1_544 . 3_564 172.8(8) no
O2 Na3 O2 7_654 . 3_564 124.1(4) no
O2 Na3 Cl1 8_454 . . 93.6(4) no
O2 Na3 Cl1 1_544 . . 93.6(4) no
O2 Na3 Cl1 7_654 . . 93.6(4) no
O2 Na3 Cl1 3_564 . . 93.6(4) no
O2 Na3 B2 8_454 . 3_565 28.60(18) no
O2 Na3 B2 1_544 . 3_565 152.30(18) no
O2 Na3 B2 7_654 . 3_565 152.30(18) no
O2 Na3 B2 3_564 . 3_565 28.60(18) no
Cl1 Na3 B2 . . 3_565 86.6(4) no
O2 Na3 B2 8_454 . 1_545 152.30(18) no
O2 Na3 B2 1_544 . 1_545 28.60(18) no
O2 Na3 B2 7_654 . 1_545 28.60(18) no
O2 Na3 B2 3_564 . 1_545 152.30(18) no
Cl1 Na3 B2 . . 1_545 86.6(4) no
B2 Na3 B2 3_565 . 1_545 173.2(7) no
O2 Na3 Ba1 8_454 . 7_665 144.1(5) no
O2 Na3 Ba1 1_544 . 7_665 80.7(2) no
O2 Na3 Ba1 7_654 . 7_665 42.3(2) no
O2 Na3 Ba1 3_564 . 7_665 103.4(3) no
Cl1 Na3 Ba1 . . 7_665 56.14(19) no
B2 Na3 Ba1 3_565 . 7_665 121.1(3) no
B2 Na3 Ba1 1_545 . 7_665 54.43(19) no
O2 Na3 Ba1 8_454 . 3_665 80.7(2) no
O2 Na3 Ba1 1_544 . 3_665 144.1(5) no
O2 Na3 Ba1 7_654 . 3_665 103.4(3) no
O2 Na3 Ba1 3_564 . 3_665 42.3(2) no
Cl1 Na3 Ba1 . . 3_665 56.14(19) no
B2 Na3 Ba1 3_565 . 3_665 54.43(19) no
B2 Na3 Ba1 1_545 . 3_665 121.1(3) no
Ba1 Na3 Ba1 7_665 . 3_665 66.71(17) no
O2 Na3 Ba1 8_454 . 1_445 103.4(3) no
O2 Na3 Ba1 1_544 . 1_445 42.3(2) no
O2 Na3 Ba1 7_654 . 1_445 80.7(2) no
O2 Na3 Ba1 3_564 . 1_445 144.1(5) no
Cl1 Na3 Ba1 . . 1_445 56.14(19) no
B2 Na3 Ba1 3_565 . 1_445 121.1(3) no
B2 Na3 Ba1 1_545 . 1_445 54.43(19) no
Ba1 Na3 Ba1 7_665 . 1_445 77.0(2) no
Ba1 Na3 Ba1 3_665 . 1_445 112.3(4) no
O2 Na3 Ba1 8_454 . 8_445 42.3(2) no
O2 Na3 Ba1 1_544 . 8_445 103.4(3) no
O2 Na3 Ba1 7_654 . 8_445 144.1(5) no
O2 Na3 Ba1 3_564 . 8_445 80.7(2) no
Cl1 Na3 Ba1 . . 8_445 56.14(19) no
B2 Na3 Ba1 3_565 . 8_445 54.43(19) no
B2 Na3 Ba1 1_545 . 8_445 121.1(3) no
Ba1 Na3 Ba1 7_665 . 8_445 112.3(4) no
Ba1 Na3 Ba1 3_665 . 8_445 77.0(2) no
Ba1 Na3 Ba1 1_445 . 8_445 66.71(17) no
B3 O1 B1 6_465 . . 122.2(10) no
B3 O1 Ba1 6_465 . 1_455 97.7(6) no
B1 O1 Ba1 . . 1_455 136.4(9) no
B3 O1 Ba1 6_465 . 4_465 102.6(6) no
B1 O1 Ba1 . . 4_465 73.3(7) no
Ba1 O1 Ba1 1_455 . 4_465 117.5(3) no
B3 O2 B2 6_465 . 1_556 119.9(8) no
B3 O2 Na3 6_465 . 1_566 103.7(7) no
B2 O2 Na3 1_556 . 1_566 98.4(6) no
B3 O2 Ba1 6_465 . 1_456 129.2(7) no
B2 O2 Ba1 1_556 . 1_456 100.6(6) no
Na3 O2 Ba1 1_566 . 1_456 98.9(4) no
Na3 Cl1 Ba1 . . 8_445 82.92(12) no
Na3 Cl1 Ba1 . . 1_445 82.92(12) no
Ba1 Cl1 Ba1 8_445 . 1_445 82.16(3) no
Na3 Cl1 Ba1 . . 3_665 82.92(12) no
Ba1 Cl1 Ba1 8_445 . 3_665 96.09(4) no
Ba1 Cl1 Ba1 1_445 . 3_665 165.8(2) no
Na3 Cl1 Ba1 . . 7_665 82.92(12) no
Ba1 Cl1 Ba1 8_445 . 7_665 165.8(2) no
Ba1 Cl1 Ba1 1_445 . 7_665 96.09(4) no
Ba1 Cl1 Ba1 3_665 . 7_665 82.16(3) no
Ba1 Cl2 Ba1 3_665 . 1_455 120.2(4) no
Ba1 Cl2 Ba1 3_665 . 4_465 106.42(2) no
Ba1 Cl2 Ba1 1_455 . 4_465 106.42(2) no
Ba1 Cl2 Ba1 3_665 . 2_545 106.42(2) no
Ba1 Cl2 Ba1 1_455 . 2_545 106.42(2) no
Ba1 Cl2 Ba1 4_465 . 2_545 110.9(3) no
B1 O5 Al2 . . . 120.4(10) no
B1 O5 Ba1 . . 6_465 85.8(6) no
Al2 O5 Ba1 . . 6_465 126.7(2) no
B1 O5 Ba1 . . 4_465 85.8(6) no
Al2 O5 Ba1 . . 4_465 126.7(2) no
Ba1 O5 Ba1 6_465 . 4_465 98.4(3) no
B2 O6 Al2 . . . 120.3(8) no
B2 O6 Ba1 . . 7_675 98.8(4) no
Al2 O6 Ba1 . . 7_675 108.4(2) no
B2 O6 Ba1 . . 1_455 98.8(4) no
Al2 O6 Ba1 . . 1_455 108.4(2) no
Ba1 O6 Ba1 7_675 . 1_455 122.6(3) no
B2 O7 B1 . . 1_554 111.3(11) no
B2 O7 Ba1 . . 4_464 125.9(3) no
B1 O7 Ba1 1_554 . 4_464 88.3(5) no
B2 O7 Ba1 . . 6_464 125.9(3) no
B1 O7 Ba1 1_554 . 6_464 88.3(5) no
Ba1 O7 Ba1 4_464 . 6_464 103.5(4) no
O5 B1 O1 . . . 111.0(9) no
O5 B1 O1 . . 7_665 111.0(9) no
O1 B1 O1 . . 7_665 110.3(14) no
O5 B1 O7 . . 1_556 108.8(13) no
O1 B1 O7 . . 1_556 107.8(9) no
O1 B1 O7 7_665 . 1_556 107.8(9) no
O5 B1 Ba1 . . 6_465 67.7(6) no
O1 B1 Ba1 . . 6_465 168.6(10) no
O1 B1 Ba1 7_665 . 6_465 80.1(5) no
O7 B1 Ba1 1_556 . 6_465 63.4(5) no
O5 B1 Ba1 . . 4_465 67.7(6) no
O1 B1 Ba1 . . 4_465 80.1(5) no
O1 B1 Ba1 7_665 . 4_465 168.6(10) no
O7 B1 Ba1 1_556 . 4_465 63.4(5) no
Ba1 B1 Ba1 6_465 . 4_465 89.2(5) no
B3 O8 Al2 . . . 138.0(7) no
B3 O8 Ba1 . . 6_464 93.7(6) no
Al2 O8 Ba1 . . 6_464 125.7(5) no
O6 B2 O7 . . . 115.2(11) no
O6 B2 O2 . . 1_554 109.2(7) no
O7 B2 O2 . . 1_554 110.4(7) no
O6 B2 O2 . . 7_664 109.2(7) no
O7 B2 O2 . . 7_664 110.4(7) no
O2 B2 O2 1_554 . 7_664 101.6(10) no
O6 B2 Na3 . . 1_565 103.7(8) no
O7 B2 Na3 . . 1_565 141.1(9) no
O2 B2 Na3 1_554 . 1_565 53.0(5) no
O2 B2 Na3 7_664 . 1_565 53.0(5) no
O6 B2 Ba1 . . 7_675 56.7(3) no
O7 B2 Ba1 . . 7_675 125.6(4) no
O2 B2 Ba1 1_554 . 7_675 123.2(7) no
O2 B2 Ba1 7_664 . 7_675 53.0(4) no
Na3 B2 Ba1 1_565 . 7_675 75.9(3) no
O6 B2 Ba1 . . 1_455 56.7(3) no
O7 B2 Ba1 . . 1_455 125.6(4) no
O2 B2 Ba1 1_554 . 1_455 53.0(4) no
O2 B2 Ba1 7_664 . 1_455 123.2(7) no
Na3 B2 Ba1 1_565 . 1_455 75.9(3) no
Ba1 B2 Ba1 7_675 . 1_455 95.8(3) no
O8 B3 O2 . . 6_564 122.3(9) no
O8 B3 O1 . . 6_564 118.7(8) no
O2 B3 O1 6_564 . 6_564 118.9(9) no
O8 B3 Ba1 . . 6_464 62.2(5) no
O2 B3 Ba1 6_564 . 6_464 172.1(8) no
O1 B3 Ba1 6_564 . 6_464 57.0(5) no
